#------------------------------------------------------------------------------
#$Date: 2016-03-23 22:13:21 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179472 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/69/4336913.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4336913
loop_
_publ_author_name
'Ikuya Yamada'
'Hidenobu Etani'
'Kazuki Tsuchida'
'Shohei Marukawa'
'Naoaki Hayashi'
'Takateru Kawakami'
'Masaichiro Mizumaki'
'Kenya Ohgushi'
'Yoshihiro Kusano'
'Jungeun Kim'
'Naruki Tsuji'
'Ryoji Takahashi'
'Norimasa Nishiyama'
'Toru Inoue'
'Tetsuo Irifune'
'Mikio Takano'
_publ_section_title
;
 Control of Bond-Strain-Induced Electronic Phase Transitions in Iron
 Perovskites
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              13751
_journal_page_last               13761
_journal_paper_doi               10.1021/ic402344m
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'Cu3 Eu Fe4 O12'
_chemical_formula_weight         757.975
_space_group_IT_number           204
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      204
_symmetry_space_group_name_Hall  '-I 2 2 3'
_symmetry_space_group_name_H-M   'I m -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.37306(8)
_cell_length_b                   7.37306(8)
_cell_length_c                   7.37306(8)
_cell_measurement_temperature    100
_cell_volume                     400.814(8)
_computing_cell_refinement       'RIETAN-FP (Izumi and Momma, 2007)'
_computing_molecular_graphics    'VESTA (Momma and Izumi, 2008)'
_computing_structure_refinement  'RIETAN-FP (Izumi and Momma, 2007)'
_diffrn_ambient_temperature      100
_diffrn_radiation_wavelength     0.420780
_diffrn_source                   synchrotron
_exptl_crystal_density_diffrn    6.2804
_exptl_crystal_F_000             700.00
_pd_calc_method                  'Rietveld Refinement'
_pd_char_colour                  grey
_pd_meas_2theta_range_inc        0.0100
_pd_meas_2theta_range_max        79.1400
_pd_meas_2theta_range_min        0.0000
_pd_meas_number_of_points        7915
_pd_meas_scan_method             step
_pd_proc_2theta_range_inc        0.0100
_pd_proc_2theta_range_max        40.0000
_pd_proc_2theta_range_min        4.0000
_pd_proc_ls_background_function  'Legendre polynomials'
_pd_proc_ls_pref_orient_corr     ' ?'
_pd_proc_ls_profile_function     'split pseudo-Voigt function'
_pd_proc_ls_prof_R_factor        0.05418
_pd_proc_ls_prof_wR_expected     0.06173
_pd_proc_ls_prof_wR_factor       0.06943
_pd_spec_mount_mode              reflection
_pd_spec_shape                   flat_sheet
_refine_diff_density_max         0.1
_refine_diff_density_min         -0.1
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   1.1247
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     29
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.00940
_refine_ls_R_Fsqd_factor         0.00861
_refine_ls_R_I_factor            0.01455
_refine_ls_shift/su_max          0.0
_refine_ls_weighting_details     1/yi
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            ic402344m_si_002_05.cif
_cod_data_source_block           single_phase
_cod_original_cell_volume        400.815(8)
_cod_database_code               4336913
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 x,y,z
2 -x,-y,z
3 -x,y,-z
4 x,-y,-z
5 z,x,y
6 z,-x,-y
7 -z,-x,y
8 -z,x,-y
9 y,z,x
10 -y,z,-x
11 y,-z,-x
12 -y,-z,x
13 -x,-y,-z
14 x,y,-z
15 x,-y,z
16 -x,y,z
17 -z,-x,-y
18 -z,x,y
19 z,x,-y
20 z,-x,y
21 -y,-z,-x
22 y,-z,x
23 -y,z,x
24 y,z,-x
25 x+1/2,y+1/2,z+1/2
26 -x+1/2,-y+1/2,z+1/2
27 -x+1/2,y+1/2,-z+1/2
28 x+1/2,-y+1/2,-z+1/2
29 z+1/2,x+1/2,y+1/2
30 z+1/2,-x+1/2,-y+1/2
31 -z+1/2,-x+1/2,y+1/2
32 -z+1/2,x+1/2,-y+1/2
33 y+1/2,z+1/2,x+1/2
34 -y+1/2,z+1/2,-x+1/2
35 y+1/2,-z+1/2,-x+1/2
36 -y+1/2,-z+1/2,x+1/2
37 -x+1/2,-y+1/2,-z+1/2
38 x+1/2,y+1/2,-z+1/2
39 x+1/2,-y+1/2,z+1/2
40 -x+1/2,y+1/2,z+1/2
41 -z+1/2,-x+1/2,-y+1/2
42 -z+1/2,x+1/2,y+1/2
43 z+1/2,x+1/2,-y+1/2
44 z+1/2,-x+1/2,y+1/2
45 -y+1/2,-z+1/2,-x+1/2
46 y+1/2,-z+1/2,x+1/2
47 -y+1/2,z+1/2,x+1/2
48 y+1/2,z+1/2,-x+1/2
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_Wyckoff_symbol
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_type_symbol
Eu1 0 0 0 1 2 a Uiso 0.0019(1) Eu
Cu1 0 0.5 0.5 1 6 b Uiso 0.0037(2) Cu
Fe1 0.25 0.25 0.25 1 8 c Uiso 0.0017(1) Fe
O1 0 0.3082(3) 0.1687(4) 1 24 g Uiso 0.0023(7) O
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Eu Eu3+ -1.2228 1.4713 'International Tables for Crystallography, Vol. C'
Cu Cu2+ 0.1908 0.4852 'International Tables for Crystallography, Vol. C'
Fe Fe3+ 0.1554 0.3160 'International Tables for Crystallography, Vol. C'
O O- -0.0011 0.0019 'International Tables for Crystallography, Vol. C'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Eu1 O1 180 1_555 4_555
O1 Eu1 O1 122.6(1) 1_555 2_555
O1 Eu1 O1 57.4(1) 1_555 3_555
O1 Eu1 O1 65.09(3) 1_555 5_555
O1 Eu1 O1 114.91(3) 1_555 8_555
O1 Eu1 O1 114.91(3) 1_555 6_555
O1 Eu1 O1 65.09(3) 1_555 7_555
O1 Eu1 O1 65.09(3) 1_555 9_555
O1 Eu1 O1 114.91(3) 1_555 12_555
O1 Eu1 O1 65.09(3) 1_555 10_555
O1 Eu1 O1 114.91(3) 1_555 11_555
O1 Eu1 O1 57.4(1) 4_555 2_555
O1 Eu1 O1 122.6(1) 4_555 3_555
O1 Eu1 O1 114.91(3) 4_555 5_555
O1 Eu1 O1 65.09(3) 4_555 8_555
O1 Eu1 O1 65.09(3) 4_555 6_555
O1 Eu1 O1 114.91(3) 4_555 7_555
O1 Eu1 O1 114.91(3) 4_555 9_555
O1 Eu1 O1 65.09(3) 4_555 12_555
O1 Eu1 O1 114.91(3) 4_555 10_555
O1 Eu1 O1 65.09(3) 4_555 11_555
O1 Eu1 O1 180 2_555 3_555
O1 Eu1 O1 65.09(3) 2_555 5_555
O1 Eu1 O1 114.91(3) 2_555 8_555
O1 Eu1 O1 114.91(3) 2_555 6_555
O1 Eu1 O1 65.09(3) 2_555 7_555
O1 Eu1 O1 114.91(3) 2_555 9_555
O1 Eu1 O1 65.09(3) 2_555 12_555
O1 Eu1 O1 114.91(3) 2_555 10_555
O1 Eu1 O1 65.09(3) 2_555 11_555
O1 Eu1 O1 114.91(3) 3_555 5_555
O1 Eu1 O1 65.09(3) 3_555 8_555
O1 Eu1 O1 65.09(3) 3_555 6_555
O1 Eu1 O1 114.91(3) 3_555 7_555
O1 Eu1 O1 65.09(3) 3_555 9_555
O1 Eu1 O1 114.91(3) 3_555 12_555
O1 Eu1 O1 65.09(3) 3_555 10_555
O1 Eu1 O1 114.91(3) 3_555 11_555
O1 Eu1 O1 180 5_555 8_555
O1 Eu1 O1 122.6(1) 5_555 6_555
O1 Eu1 O1 57.4(1) 5_555 7_555
O1 Eu1 O1 65.09(3) 5_555 9_555
O1 Eu1 O1 114.91(3) 5_555 12_555
O1 Eu1 O1 114.91(3) 5_555 10_555
O1 Eu1 O1 65.09(3) 5_555 11_555
O1 Eu1 O1 57.4(1) 8_555 6_555
O1 Eu1 O1 122.6(1) 8_555 7_555
O1 Eu1 O1 114.91(3) 8_555 9_555
O1 Eu1 O1 65.09(3) 8_555 12_555
O1 Eu1 O1 65.09(3) 8_555 10_555
O1 Eu1 O1 114.91(3) 8_555 11_555
O1 Eu1 O1 180 6_555 7_555
O1 Eu1 O1 65.09(3) 6_555 9_555
O1 Eu1 O1 114.91(3) 6_555 12_555
O1 Eu1 O1 114.91(3) 6_555 10_555
O1 Eu1 O1 65.09(3) 6_555 11_555
O1 Eu1 O1 114.91(3) 7_555 9_555
O1 Eu1 O1 65.09(3) 7_555 12_555
O1 Eu1 O1 65.09(3) 7_555 10_555
O1 Eu1 O1 114.91(3) 7_555 11_555
O1 Eu1 O1 180 9_555 12_555
O1 Eu1 O1 122.6(1) 9_555 10_555
O1 Eu1 O1 57.4(1) 9_555 11_555
O1 Eu1 O1 57.4(1) 12_555 10_555
O1 Eu1 O1 122.6(1) 12_555 11_555
O1 Eu1 O1 180 10_555 11_555
O1 Cu1 O1 82.7(2) 36_555 34_555
O1 Cu1 O1 180.0000(2) 36_555 33_455
O1 Cu1 O1 97.3(2) 36_555 35_455
O1 Cu1 O1 70.67(4) 36_555 1_555
O1 Cu1 O1 109.33(4) 36_555 2_565
O1 Cu1 O1 70.67(4) 36_555 3_556
O1 Cu1 O1 109.33(4) 36_555 4_566
O1 Cu1 O1 97.3(2) 34_555 33_455
O1 Cu1 O1 109.33(4) 34_555 1_555
O1 Cu1 O1 70.67(4) 34_555 2_565
O1 Cu1 O1 109.33(4) 34_555 3_556
O1 Cu1 O1 70.67(4) 34_555 4_566
O1 Cu1 O1 82.7(2) 33_455 35_455
O1 Cu1 O1 109.33(4) 33_455 1_555
O1 Cu1 O1 70.67(4) 33_455 2_565
O1 Cu1 O1 109.33(4) 33_455 3_556
O1 Cu1 O1 70.67(4) 33_455 4_566
O1 Cu1 O1 70.67(4) 35_455 1_555
O1 Cu1 O1 109.33(4) 35_455 2_565
O1 Cu1 O1 70.67(4) 35_455 3_556
O1 Cu1 O1 109.33(4) 35_455 4_566
O1 Cu1 O1 60.1(1) 1_555 2_565
O1 Cu1 O1 119.9(1) 1_555 3_556
O1 Cu1 O1 180.0000(1) 1_555 4_566
O1 Cu1 O1 180.0000(1) 2_565 3_556
O1 Cu1 O1 119.9(1) 2_565 4_566
O1 Cu1 O1 60.1(1) 3_556 4_566
O1 Fe1 O1 180 1_555 28_555
O1 Fe1 O1 89.2(1) 1_555 5_555
O1 Fe1 O1 90.8(1) 1_555 32_555
O1 Fe1 O1 89.2(1) 1_555 9_555
O1 Fe1 O1 90.8(1) 1_555 36_555
O1 Fe1 O1 90.8(1) 28_555 5_555
O1 Fe1 O1 89.2(1) 28_555 32_555
O1 Fe1 O1 90.8(1) 28_555 9_555
O1 Fe1 O1 89.2(1) 28_555 36_555
O1 Fe1 O1 180 5_555 32_555
O1 Fe1 O1 89.2(1) 5_555 9_555
O1 Fe1 O1 90.8(1) 5_555 36_555
O1 Fe1 O1 90.8(1) 32_555 9_555
O1 Fe1 O1 89.2(1) 32_555 36_555
O1 Fe1 O1 180 9_555 36_555
Cu1 O1 Fe1 111.20(7) 29_454 1_555
Cu1 O1 Fe1 111.20(7) 29_454 16_555
Cu1 O1 O1 48.67(8) 29_454 3_555
Cu1 O1 Eu1 110.0(1) 29_454 1_555
Cu1 O1 O1 148.8(1) 29_454 5_555
Cu1 O1 O1 148.8(1) 29_454 7_555
Cu1 O1 O1 89.0(1) 29_454 9_555
Cu1 O1 O1 89.0(1) 29_454 10_555
Cu1 O1 Cu1 101.3(1) 29_454 1_555
Cu1 O1 O1 70.38(3) 29_454 32_555
Cu1 O1 O1 121.7(1) 29_454 36_555
Cu1 O1 O1 70.38(3) 29_454 30_455
Cu1 O1 O1 121.7(1) 29_454 35_455
Cu1 O1 O1 41.33(8) 29_454 2_565
Fe1 O1 Fe1 136.4(1) 1_555 16_555
Fe1 O1 O1 107.57(8) 1_555 3_555
Fe1 O1 Eu1 87.45(7) 1_555 1_555
Fe1 O1 O1 45.41(5) 1_555 5_555
Fe1 O1 O1 97.3(1) 1_555 7_555
Fe1 O1 O1 45.41(5) 1_555 9_555
Fe1 O1 O1 144.30(9) 1_555 10_555
Fe1 O1 Cu1 81.20(8) 1_555 1_555
Fe1 O1 O1 44.59(5) 1_555 32_555
Fe1 O1 O1 44.59(5) 1_555 36_555
Fe1 O1 O1 153.1(1) 1_555 30_455
Fe1 O1 O1 102.5(1) 1_555 35_455
Fe1 O1 O1 102.48(7) 1_555 2_565
Fe1 O1 O1 107.57(8) 16_555 3_555
Fe1 O1 Eu1 87.45(7) 16_555 1_555
Fe1 O1 O1 97.3(1) 16_555 5_555
Fe1 O1 O1 45.41(5) 16_555 7_555
Fe1 O1 O1 144.30(9) 16_555 9_555
Fe1 O1 O1 45.41(5) 16_555 10_555
Fe1 O1 Cu1 81.20(8) 16_555 1_555
Fe1 O1 O1 153.1(1) 16_555 32_555
Fe1 O1 O1 102.5(1) 16_555 36_555
Fe1 O1 O1 44.59(5) 16_555 30_455
Fe1 O1 O1 44.59(5) 16_555 35_455
Fe1 O1 O1 102.48(7) 16_555 2_565
O1 O1 Eu1 61.30(6) 3_555 1_555
O1 O1 O1 111.65(7) 3_555 5_555
O1 O1 O1 111.65(7) 3_555 7_555
O1 O1 O1 63.49(7) 3_555 9_555
O1 O1 O1 63.49(7) 3_555 10_555
O1 O1 Cu1 149.93(5) 3_555 1_555
O1 O1 O1 93.45(7) 3_555 32_555
O1 O1 O1 149.75(5) 3_555 36_555
O1 O1 O1 93.45(7) 3_555 30_455
O1 O1 O1 149.75(5) 3_555 35_455
O1 O1 O1 90 3_555 2_565
Eu1 O1 O1 57.46(2) 1_555 5_555
Eu1 O1 O1 57.46(2) 1_555 7_555
Eu1 O1 O1 57.46(2) 1_555 9_555
Eu1 O1 O1 57.46(2) 1_555 10_555
Eu1 O1 Cu1 148.8(1) 1_555 1_555
Eu1 O1 O1 117.88(6) 1_555 32_555
Eu1 O1 O1 117.88(6) 1_555 36_555
Eu1 O1 O1 117.88(6) 1_555 30_455
Eu1 O1 O1 117.88(6) 1_555 35_455
Eu1 O1 O1 151.30(6) 1_555 2_565
O1 O1 O1 53.0(1) 5_555 7_555
O1 O1 O1 60 5_555 9_555
O1 O1 O1 103.17(9) 5_555 10_555
O1 O1 Cu1 95.12(9) 5_555 1_555
O1 O1 O1 90 5_555 32_555
O1 O1 O1 60.47(6) 5_555 36_555
O1 O1 O1 140.5(1) 5_555 30_455
O1 O1 O1 87.3(1) 5_555 35_455
O1 O1 O1 144.614(7) 5_555 2_565
O1 O1 O1 103.17(9) 7_555 9_555
O1 O1 O1 60 7_555 10_555
O1 O1 Cu1 95.12(9) 7_555 1_555
O1 O1 O1 140.5(1) 7_555 32_555
O1 O1 O1 87.3(1) 7_555 36_555
O1 O1 O1 90 7_555 30_455
O1 O1 O1 60.47(6) 7_555 35_455
O1 O1 O1 144.614(7) 7_555 2_565
O1 O1 O1 109.23(1) 9_555 10_555
O1 O1 Cu1 124.83(3) 9_555 1_555
O1 O1 O1 60.47(6) 9_555 32_555
O1 O1 O1 90 9_555 36_555
O1 O1 O1 156.3(1) 9_555 30_455
O1 O1 O1 144.6(1) 9_555 35_455
O1 O1 O1 111.65(7) 9_555 2_565
O1 O1 Cu1 124.83(3) 10_555 1_555
O1 O1 O1 156.3(1) 10_555 32_555
O1 O1 O1 144.6(1) 10_555 36_555
O1 O1 O1 60.47(6) 10_555 30_455
O1 O1 O1 90 10_555 35_455
O1 O1 O1 111.65(7) 10_555 2_565
Cu1 O1 O1 72.38(8) 1_555 32_555
Cu1 O1 O1 38.95(7) 1_555 36_555
Cu1 O1 O1 72.38(8) 1_555 30_455
Cu1 O1 O1 38.95(7) 1_555 35_455
Cu1 O1 O1 59.93(5) 1_555 2_565
O1 O1 O1 59.1(1) 32_555 36_555
O1 O1 O1 119.5(1) 32_555 30_455
O1 O1 O1 110.5(1) 32_555 35_455
O1 O1 O1 59.99(5) 32_555 2_565
O1 O1 O1 110.5(1) 36_555 30_455
O1 O1 O1 60.0(1) 36_555 35_455
O1 O1 O1 86.55(7) 36_555 2_565
O1 O1 O1 59.1(1) 30_455 35_455
O1 O1 O1 59.99(5) 30_455 2_565
O1 O1 O1 86.55(7) 35_455 2_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Eu1 O1 2.591(3) 1_555
Eu1 O1 2.591(3) 4_555
Eu1 O1 2.591(3) 2_555
Eu1 O1 2.591(3) 3_555
Eu1 O1 2.591(3) 5_555
Eu1 O1 2.591(3) 8_555
Eu1 O1 2.591(3) 6_555
Eu1 O1 2.591(3) 7_555
Eu1 O1 2.591(3) 9_555
Eu1 O1 2.591(3) 12_555
Eu1 O1 2.591(3) 10_555
Eu1 O1 2.591(3) 11_555
Cu1 O1 1.884(3) 36_555
Cu1 O1 1.884(3) 34_555
Cu1 O1 1.884(3) 33_455
Cu1 O1 1.884(3) 35_455
Cu1 O1 2.822(3) 1_555
Cu1 O1 2.822(3) 2_565
Cu1 O1 2.822(3) 3_556
Cu1 O1 2.822(3) 4_566
Fe1 O1 1.9851(9) 1_555
Fe1 O1 1.9851(9) 28_555
Fe1 O1 1.9851(9) 5_555
Fe1 O1 1.9851(9) 32_555
Fe1 O1 1.9851(9) 9_555
Fe1 O1 1.9851(9) 36_555
O1 Cu1 1.884(3) 29_454
O1 Fe1 1.9851(9) 1_555
O1 Fe1 1.9851(9) 16_555
O1 O1 2.488(5) 3_555
O1 Eu1 2.591(3) 1_555
O1 O1 2.787(3) 5_555
O1 O1 2.787(3) 7_555
O1 O1 2.787(3) 9_555
O1 O1 2.787(3) 10_555
O1 Cu1 2.822(3) 1_555
O1 O1 2.828(3) 32_555
O1 O1 2.828(3) 36_555
O1 O1 2.828(3) 30_455
O1 O1 2.828(3) 35_455
O1 O1 2.829(5) 2_565
